SYNTHESIS OF β-TCP POWDER VIA WET PRECIPITATION...
Embed Size (px)
Transcript of SYNTHESIS OF β-TCP POWDER VIA WET PRECIPITATION...
SYNTHESIS OF -TCP POWDER VIA
WET PRECIPITATION AND HYDROTHERMAL METHODS
PHAM TRUNG KIEN
UNIVERSITI SAINS MALAYSIA
SYNTHESIS OF -TCP POWDER VIA WET PRECIPITATION AND HYDROTHERMAL METHODS
PHAM TRUNG KIEN
Thesis submitted in fulfillment of the requirements for the degree
of Master of Science
Saya isytiharkan bahawa kandungan yang dibentangkan di dalam tesis ini
adalah hasil kerja saya sendiri dan telah dijalankan di Universiti Sains Malaysia
kecuali dimaklumkan sebaliknya. Tesis ini juga tidak pernah disertakan untuk
ijazah yang lain sebelum ini.
Disaksikan Oleh: Tandatangan Calon Tandatangan Penyelia/Dekan Nama Calon: Pham Trung Kien
I would like to express my most sincere thanks that come deeply from my heart
to those who made this research study possible.
Firstly, I want to acknowledge my main supervisor Prof. Radzali Othman and
my co-supervisor Assoc. Prof. Dr. Ahmad Fauzi Mooh for their help and advice on my
research. I am also grateful to Assoc. Prof. Dr. Khairun Azizi Azizli and the staff of the
School of Materials and Mineral Resources Engineering, Universiti Sains Malaysia, for
their kindness and support.
This work would not have been possible without the financial support from
AUN-SEED Net/JICA. I would like to deliver my sincere thanks and deepest gratitude
for their generosity on giving me this opportunity and financial support pursuing my
My special thanks and appreciation are also extended to those people who in
one way or another helped me accomplish this research:
To Madam Fong Lee Lee, Mr. Kemuridan for their kindness, help, and
assistance; to Mr. Rashid, and Mr. Karuna for their help in conducting SEM and XRD;
To Prof. Kunio Ishikawa from the Department of Biomaterials, Faculty of Dental
Science, Kyushu University, Japan for his advice on my study, and in living;
To Dr. Do Quang Minh, my co-advisor from the Department of Silicate
Materials, Faculty of Materials Technology, Ho Chi Minh University of Technology, for
his help and support.
To all my friends ( Long, Quynh and Umar) for their help and friendship.
To my family for their understanding support and inspiration.
TABLE OF CONTENTS
Table of Contents iii
List of Tables vii
List of Figures ix
List of Abbreviations xii
CHAPTER 1: INTRODUCTION
1.1 Introduction 1
1.2 Problem statement 2
1.3 Objectives of research 4
1.4 Research scope 5
CHAPTER 2: LITERATURE REVIEW
2.1 Biomaterials 8
2.2 Types of synthetic biomaterials 10
2.2.1 Metallic biomaterials 10
2.2.2 Ceramic and glass biomaterials 11
2.2.3 Polymeric biomaterials 15
2.3 Calcium phosphate ceramics (CPC) 17
2.3.1 General properties of calcium phosphate ceramics 17
2.3.2 Hydroxyapatie 21
2.3.3 Tricalcium phosphate (TCP 22
2.3.4 Trace element measurement of HA and -TCP for surgical implant 24
2.3.5 Thermal behaviour of calcium phosphate ceramic 24
2.4 Previous study on synthesis -TCP 27
2.4.1 Solid-state reactions 27
2.4.2 Wet chemical reactions 31
2.5 Powder synthesis method 38
2.5.1 The wet precipitation method 38
2.5.2 Hydrothermal method 39
CHAPTER 3: MATERIALS AND METHODS
3.1 Starting materials and solution preparation 41
3.1.1 Starting materials 41
3.1.2 Solution preparation 42
188.8.131.52 Preparation of 0.3 mole H3PO4 solution (solution A1) 43
184.108.40.206 Preparation of 0.45 mole calcium hydroxide solution
(solution A2) 43
3.2 Experimental method 44
3.2.1 The wet precipitation method 44
220.127.116.11 Effect of different stirring speeds 48
18.104.22.168 Effect of different calcination temperatures 49
22.214.171.124 Effect of different calcination soaking times 49
126.96.36.199 Effect of different stirring durations 50
3.2.2 Hydrothermal method 51
188.8.131.52 Effect of different stirring speeds 51
184.108.40.206 Effect of different calcination temperatures 54
3.3 Trace element measurement of -TCP powder for surgical implant 54
3.4 Characterization 55
3.4.1 Thermal analysis (DSC/TG) 55
3.4.2 X-Ray Powder Diffraction (XRD) 56
3.4.3 Fourier Transform Infrared (FTIR) spectroscopy 57
3.4.4 Scanning electron microscopy (SEM) 58
3.4.5 Powder density measurement 59
3.4.6 Trace element measurement 60
CHAPTER 4: RESULTS AND DISCUSSION
4.1 Characterization of starting materials 62
4.1.1 XRD analysis 62
4.1.2 Thermal analysis 63
4.1.3 Morphological analysis 64
4.2 Synthesis of -TCP powder using the wet precipitation method 64
4.2.1 Effect of different stirring speeds 65
220.127.116.11 pH measurement 65
18.104.22.168 Thermal analysis: 66
22.214.171.124 XRD analysis 70
126.96.36.199 Evidence of reproducibility 77
188.8.131.52 FTIR analysis 78
4.2.2 Effect of different calcination temperatures 80
184.108.40.206 XRD analysis 80
220.127.116.11 Morphological analysis and density measurement 87
4.2.3 Effect of different calcination soaking times 90
18.104.22.168 XRD analysis 90
22.214.171.124 Morphological analysis and density measurement 92
4.2.4 Effect of different stirring durations 94
126.96.36.199 pH measurement 94
188.8.131.52 Thermal analysis: 95
184.108.40.206 XRD analysis 98
220.127.116.11 FTIR analysis 101
18.104.22.168 Morphological analysis and density measurement 103
4.3 Synthesis of -TCP using hydrothermal method 106
4.3.1 Effect of different stirring speeds 106
22.214.171.124 pH measurement 106
126.96.36.199 Thermal analysis 107
188.8.131.52 XRD analysis 110
184.108.40.206 FTIR analysis 112
4.3.2 Effect of different calcination temperatures 114
220.127.116.11 XRD analysis 114
18.104.22.168 Morphological analysis 115
4.4 Trace element measurement of -TCP powder for surgical implant 117
4.5 Summary 118
CHAPTER 5: CONCLUSIONS
5.1 Conclusions 119
5.2 Suggestions for future work 120
Appendix A Solution calculation
Appendix B Calculation on the loss of lattice water of Ca(OH)2
Appendix C ICDD card of XRD pattern
Appendix D XRD patterns
LIST OF PUBLICATIONS 151
LIST OF TABLES
1.1 Prediction of market share of orthopedic biomaterials over the world
in 5 years 2007-2011.
2.1 Classification of biomaterials. 9
2.2 Selected properties of metallic biomaterials. 11
2.3 Ceramics used in biomedical application. 13
2.4 Mechanical properties of ceramic biomaterial. 15
2.5 Examples of biomedical application of polymers. 16
2.6 Mechanical properties of biomedical polymers. 17
2.7 Comparison between enamel, dentin, bone and synthetic apatite. 18
2.8 Various phases of calcium phosphate ceramics. 19
2.9 Solubility of different calcium phosphates. 19
2.10 Physical properties of calcium phosphates. 19
2.11 Calcium phosphates used for direct tablet. 20
2.12 Standard specification of HA and -TCP for surgical implant. 24
2.13 Combinations and compositions of the raw materials for reaction
2.14 Crystalline phase of reaction-sintered bodies using various
combinations of the raw materials.
2.15 The summary of previous study on synthesis -TCP. 36
3.1 Trace elements in calcium hydroxide. 41
3.2 Trace elements in phosphoric acid. 42
3.3 Batch code employed for different stirring speeds. 48
3.4 Batch code employed for different stirring durations. 50
3.5 Batch code employed for different stirring speeds. 52
3.6 Standard specification of -TCP for surgical implant 54
4.1 pH value of mixtures before and after reaction. 65
4.2 Tabulation of DSC/TG results for as-prepared S0, S100, S200, S300
and S400 powder.
4.3 Summary of the phase(s) in the as-prepared S0, S100, S200, S300
and S400 powders and the corresponding strongest intensity
positions on 2 axis.
4.4 Summary of the phase(s) in S0, S100, S200, S300 and S400
powders calcined at 900oC and the corresponding strongest intensity
positions on 2 axis.
4.5 FTIR peaks of S0, S100, S200, S300 and S400 filter liquid. 80
4.6 The effect of calcination temperature on the phase transformation of
4.7 Comparison of XRD data of powder calcined at different temperature
with -TCP standard pattern (ICDD 9-169).
4.8 The effect of calcination temperature on the crystallite size of -TCP
powder along (0 2 10) direction.
4.9 Summary of the effect of calcination temperature on the morphology
of S200 powder.
4.10 The 2 and relative intensity of S200 powder calcined at 900oC with
different soaking times compared to standard -TCP (ICDD card 9-
4.11 Crystallite size and grain size of powders calcined at 900oC with
different soaking times.
4.12 Grain size and density of powders calcined at 900oC with different
4.13 pH value of four different mixtures before and after reaction. 95
4.14 Tabulation of DSC/TG for T1, S200, T3 and T4 powder. 98
4.15 Phase identification of T1, S200, T3 and T4 powders calcined at
900oC for 1 hour soaking time.
4.16 The FTIR peaks of filtrated liquid of T1, S200, T3 and T4. 102
4.17 Summary of the effect of different stirring times on the morphology of
powders calcined at 900oC for 1 hour.
4.18 Summary of properties of synthesized -TCP powder at different
reaction and calcination parameters.
4.19 pH value of three different mixtures before and after hydrothermal
4.20 Tabulation of DSC/TG curves for as-prepared H0, H50 and H100
4.21 The FTIR peaks of filtered liquid of H0, H50 and H100 sample. 113
4.22 The concentration of Pb, As and Cd element in liquid and in powder
LIST OF FIGURES
1.1 Flow chart of the wet precipitation method (the first part) 6
1.2 Flow chart of the hydrothermal method (the second part) 7
2.1 Bioactivity spectrum for various bioceramic implants. 14
2.2 Differential thermal analysis curves of (1) brushite, (2) MCP, (3)
monetite and (4) Hydroxyapatite.
2.3 XRD patterns of 8 hours mechanically milled (a) as-prepared -TCP
and -TCP powder calcined at (b) 300oC, (c) 600oC and (d) 900oC in
stagnant air for 10 hours.
2.4 XRD patterns of synthesized powder calcined at 900oC, derived from
(a): 1:1.1 ratio, (b) 1:1.3 ratio, (c) 1:1.5 ratio and (d) 1:1.7 ratio (wt. %
of eggshell : phosphoric acid).
2.5 XRD patterns of sintered bodies using various combinations of the
raw materials (sintering condition: 1100oC, 24 hours, in air)
2.6 XRD patterns of coating layers with different number of deposition
(1c coating, 5c coating and 10c coating). Maxima attributable to -
TCP are indexed; (*) are Al2O3 peak
2.7 XRD patterns of TCP precipitates (A) as-dried, (B) calcined at 800oC
and (C) calcined at 1200oC for 2 hours
2.8 Effect of temperature on the crystallization of the TCP precursor as
followed by XRD: (a) XRD patterns from
100oC to 750oC and (b) XRD patterns from 800oC to 1120oC
2.9 XRD patterns of -TCP obtained at different temperatures for 2
hours: (A) 800oC, (B) 850oC, (C) 950oC, (D) 1050oC, (E) 1150oC,
2.10 Processing flow diagram for the preparation of a pure precipitate 39
3.1 Materials and laboratory tools for the preparation of solution A1 and
3.2 Experimental set up for the wet precipitation method. 45
3.3 Flow chart of the wet precipitation method. 47
3.4 High-pressure batch reactor. 51
3.5 Flow chart of hydrothermal method producing -TCP 53
3.6 X-ray diffratometer (D5000 Siemens) 57
3.7 Fourier Transform Infrared Spectrophotometer 58
3.8 SEM Model Leo Supre 35VP. 59
3.9 AccuPyc 1330 Pycnometer 60
4.1 XRD pattern for pure Ca(OH)2 starting powder 62
4.2 DSC/TG curves for calcium hydroxide. 63
4.3 SEM morphology of Ca(OH)2 at different magnifications of:
(a) 5,000 X (b) 15,000 X
4.4 DSC/TG curves for as-prepared powders:
a) S0 b) S100 c) S200 d) S300 and e) S400
4.5 XRD patterns of as-prepared powders (bottom) and powders
calcined at 900oC (top) for 2 hours soaking time:
a) S0 b) S100 c) S200 d) S300 and e) S400.
4.6 XRD patterns of S200-1 powders of: a) as-prepared b) 900oC 78
4.7 FTIR spectra of filtered liquid: a) S0 b) S100 c) S200
d) S300 and e) S400.
4.8 XRD patterns of S200 powder calcined at different temperatures for
2 hours soaking time:
a) as-prepared powder b) 500oC c) 700oC and d) 900oC
4.9 Difference in single crystallite and polycrystallite powder 87
4.10 SEM morphology of S200 powder calcined at 900oC for 2 hours at
different magnifications: a) 5,000 X and b) 15,000X
4.11 SEM morphology of S200 powder calcined at 1000oC for 2 hours at
different magnifications: a) 5,000 X and b) 15.000 X
4.12 SEM morphology of S200 powder calcined at 1100oC for 2 hours at
different magnifications: a) 5,000 X and b) 15,000 X
4.13 SEM morphology of S200 powder calcined at different temperatures
for 2 hours at magnification 5,000 X: (a) 1200oC (b) 1300oC
4.14 XRD patterns of S200 powder calcined at 900oC with different
soaking times. All peaks are assigned for -TCP:
a) 1 hour b) 2 hours c) 3 hours and d) 4 hours
4.15 SEM morphology of S200 powder calcined at 900oC with different
soaking times at magnification 15,000 X
a) 1 hour b) 2 hours c) 3 hours and d) 4 hours.
4.16 DSC/TG curves for as-prepared powder at different stirring
durations: a) T1 b) S200 c) T3 and d) T4
4.17 XRD patterns of as-prepared powder (bottom) and powder calcined
at 900oC for 1 hour (top): a) T1 b) S200 c) T3 and d) T4.
4.18 FTIR spectra of filtered liquid of: a) T1 b) S200 c) T3 and d) T4. 102
4.19 SEM morphology of powders calcined at 900oC for 1 hour:
a) S200 b) T3 and c) T4.
4.20 DSC/TG curves of as-prepared powder: a) H0 b) H50 and c) H100 109
4.21 XRD patterns of as-prepared powder (bottom) and powder calcined
at 900oC for 1 hour (top): a) H0 b) H50 and c) H100
4.22 FTIR spectra of filtered liquid a) H0 b) H50 and c) H100 113
4.23 XRD patterns of H0 powders calcined at different temperatures for 1
hour: a) as-prepared b) 300oC c) 500oC d) 700oC and e) 900oC
4.24 SEM morphology of powder calcined at 900oC for 1 hour at different
magnification: a) 5,000X and b) 15,000 X
LIST OF ABBREVIATION CF : Carbon fiber
CPC : Calcium phosphate ceramics
DCP : Dicalcium phosphate
DCPA : Dicalcium phosphate anhydrous
DCPD : Dicalcium phosphate dihydrate
DSC : Differential scanning calorimetry
FTIR : Fourier transform infrared
HA : Hydroxyapatite
ICP : Inductively coupled plasma
MCP : Monocalcium phosphate monohydrate
nm : nanometer
PEEK : Polyethyletheketone
PMMA : Polymethylmethacarylate
ppm : Part per million
PTFE : Polytetrafluoroethylene
PU : Polyurethane
PVC : Polyvinylchloride
rpm : Round per minute
SEM : Scanning electron microscope
STA : Simultaneous thermal analysis
TCP : Tricalcium phosphate
TG : Thermogravimetry
UHMWPE : Ultra High Molecular Weight Polyethylene
XRD : X-ray diffraction
m : Micrometer
SINTESIS SERBUK -TCP
MELALUI KAEDAH PEMENDAKAN BASAH DAN HIDROTERMA.
Matlamat kajian ini adalah untuk mensintesis -TCP [-Ca3(PO4)2] menggunakan
Ca(OH)2 dan H3PO4 sebagai bahan mula. Dua pendekatan telah digunakan dalam
kajian ini untuk menghasilkan -TCP, iaitu kaedah pemendakan basah dan kaedah
hidtroterma. Kajian ini telah mengesahkan bahawa kesan kelajuan pengadukan
memainkan peranan yang lebih penting berbanding tempoh pengadukan. Keadaan
optimum untuk menghasilkan serbuk -TCP fasa tunggal adalah : (1) kelajuan
pengadukan : 200rpm ; (2) tempoh pengadukan: 2 jam ; (3) suhu kalsin : 900oC
dengan tempoh rendam 1 jam. Lebih penting, kajian ini telah membuktikan bahawa
fasa dalam serbuk sebelum kalsin untuk mendapatkan -TCP fasa tunggal adalah
campuran fasa monetit [CaHPO4] dan hidrosiapatit [Ca10(PO4)6(OH)2].
Berdasarkan kajian pemendakan, kaedah hidroterma telah digunakan untuk
mensintesis -TCP menggunakan Ca(OH)2 dan H3PO4 sebagai bahan mula. Analisis
XRD menunjukkan serbuk yang dihasilkan mempunyai fasa campuran brushite
[CaHPO4.2H2O] dan HA berbanding dengan fasa campuran monetit dan HA dari
kaedah pemendakan. Serbuk kemudian dikalsin pada suhu 900oC selama 1 jam. XRD
mengesahkan bahawa serbuk -TCP fasa tunggal telah berjaya dihasilkan.
Namun, ketumpatan -TCP yang diperolehi daripada kaedah pemendakan
adalah 3.1g/cm3, (hampir sama dengan nilai -TCP komersil (=3.17g/cm3)) manakala
kaedah hidroterma menghasilkan serbuk yang mempunyai ketumpatan lebih tinggi
(iaitu sekitar 3.7 g/cm3). Ini dipercayai berpunca daripada pemampatan (sebelum
kalsin) dan seterusnya pensinteran (selepas kalsin) serbuk kepada butir-butir bersaiz
seragam sewaktu sintesis. Tambahan pula, serbuk -TCP yang disintesis
menggunakan kedua-dua kaedah didapati telah menepati keperluan Piawaian implan
pembedahan ASTM F1088-04a dengan kandungan toksik yang sangat rendah.
SYNTHESIS OF -TCP POWDER
VIA WET PRECIPITATION AND HYDROTHERMAL METHODS.
The purpose of this study is to synthesize -TCP [-Ca3(PO4)2] using Ca(OH)2
and H3PO4 as the starting material. Two approaches were used in this work to produce
-TCP, namely a precipitation method and a hydrothermal method. This research work
reveals that the effect of stirring speed plays significant role than that of stirring
duration. The optimum conditions to produced a single-phase -TCP are: (1) stirring
speed of 200 rpm; (2) stirring duration of 2 hours; (3) calcination temperature of 900oC
for 1 hour soaking time. Since -TCP cannot be directly precipitated from aqueous
solution, it was found that the most optimum precursor phase(s) in the as-prepared
powder to produce -TCP after calcination is a mixture phase of monetite [CaHPO4]
and hydroxyapatite [Ca10(PO4)6(OH)2].
Based on the precipitation study, a hydrothermal method was used to
synthesize -TCP using Ca(OH)2 and H3PO4 as the starting materials in a high-
pressure reactor. XRD study shows that the as-prepared powder is a mixture phase of
brushite [CaHPO4.2H2O] and HA instead of monetite and HA as found in the
precipitation method. The powder was then calcined at 900oC for 1 hour and it was
found that a single-phase -TCP was also successfully produced.
The density of -TCP obtained by the precipitation method is around 3.1g/cm3
(almost similar to a commercial -TCP (=3.17g/cm3)) whilst the hydrothermal method
produced powders of higher density (density around 3.7 g/cm3). This is attributed to the
packing and sintering of the powder into uniformly-sized grains during synthesis. In
addition, the -TCP powders synthesized using both methods satisfy the requirements
of the Standard for surgical implant, via ASTM F1088-04a with a very low level of toxic
1.1 Introduction Biomaterials are the emerging fields that are growing rapidly to fulfill the
demand in medicine and dentistry. Over the past few decades, new
biomaterials for bone replacement, total hip prosthesis and dental implants have
been synthesized and commercialized for various needs. Currently, thousands
of these materials can be found easily in the market. The market for orthopedic
biomaterials over the world is worth over US$25 billion in 2006 and with a
growth rate of more than 5% a year (refer Table 1.1). The market for orthopedic
biomaterials is expected to increase each year due to the need for better
solution for injuries, diseases and ageing population all over the world.
Table 1. 1: Prediction of market share of orthopedic biomaterials over the
world in five years from 2007 to 2011 (Driscoll, 2006).
Year Worldwide sales (US$ Billions) Growth (%)
2007 27.122 5.3
2008 28.562 5.3
2009 30.989 8.5
2010 31.708 2.5
2011 33.425 5.4
Average growth rate (%) 5.4
However, none of orthopedic biomaterials provides a perfect solution for
guiding bone healing, because there always remain the questions about
mechanical stability, long term in-vivo biocompatibility and biodegradability, the
study on orthopedic biomaterials increases every year (Tadic and Beckmann,
1.2 Problem statement
The orthopedic biomaterials market consists primarily of bone graft
substitutes, bone growth factors, degradable tissue fixation and tissue
technologies for cartilage regeneration. Generally, orthopedic prostheses
should offer a functional life of at least 20 years to match the life span of most
patients. This presents a considerable problem for most orthopedic biomaterial
(Batchelor and Chandrasekaran, 2004).
In Malaysia, orthopedic biomaterial researches especially on bone graft
and degradable materials are still in the infancy stage. Up to now, Malaysia has
spent more than RM20 million each year to buy synthetic bone graft from
foreign countries such as Switzerland, Germany and the United States.
Therefore, the Malaysian government intends to produce bone graft of it own
with the supporting research from Universiti Sains Malaysia (USM), Malaysian
Institute for Nuclear Technology Research (MINT), Universiti Kebangsaan
Malaysia (UKM) and International Islamic University Malaysia (IIUM). (Material
Medical Malaysian website, 2006).
Due to the high demands for bone substitutes, many researches have
been conducted to produce synthetic bone substitutes in large quantities as
reported by Jinawath et al., (2002), Saeri et al.,(2003), Kondo et al., (2005),
Murugan et al., (2006) and Horch et al., (2006). Synthetic bone graft materials
such as ceramics, polymers and metals were introduced as an alternative to the
traditional bone substitute. Among these materials, calcium phosphate ceramics
such as hydroxyapatite (HA) and -Tricalcium phosphate (-TCP) are the most
suitable materials with excellent biological properties. There are not so many
researches up to date that have been done on the synthesis of -TCP. Most of
the researches focused on synthesis of HA powders or biphasic HA/-TCP
powder such as Zhang et al., (2001), Anee et al., (2003), Liu et al., (2003),
Murugan and Ramakrishna (2003) and Cheng et al., (2006). However, the
interest on -TCP increases in recent years due to the high competition in
producing bone graft in the market share of orthopedic biomaterial. Generally -
TCP was prepared by a solid-state reaction and a wet chemical reaction. The
solid state reaction was reported by Lee et al., (2007), Choi and Kumta (2007),
and Yoshida et al., (2007) whilst the wet chemical reaction was carried out by
Koc (2004), Vallet-Regi et al., (2004), Zou et al., (2005) and Kwon et al., (2006)
(all of these methods will be discussed later in chapter 2). These synthesized -
TCP powders were not stable in term of thermal properties whereby they were
converted to -TCP at temperature above 1125oC.
The present research modified the study of Cheang and Khor (1995),
Saeri et al., (2003), Afshar et al., (2003) and Nagai and Nishimura, (1980) to
synthesize -TCP. According to Saeri et al., (2003) and Afshar et al., (2003),
HA can be synthesized by using the system of Ca(OH)2 and H3PO4 with a Ca/P
ratio of 1.67. This reaction was expected to be developed towards an industrial-
scale method to produce HA with the correct stoichiometric composition,
according to the Equation (1.1):
10Ca(OH)2 + 6H3PO4 Ca10(PO4)6(OH)2 + 18H2O (1.1)
The advantages of this reaction are:
The reaction involves no foreign elements
The only by-product of the reaction is water
In the present research work, a wet chemical reaction such as the
precipitation method and also the hydrothermal method were carried out to
prepare -TCP. Instead of using a Ca/P ratio of 1.67, a modification was
attempted whereby Ca(OH)2 and H3PO4 were use as starting materials with a
Ca/P ratio of 1.5. The mechanism of phase transformation in both of these
synthesis methods were fully explored.
1.3 Objectives of research
This study is focused on certain variables such as reaction parameters
(stirring speed and stirring duration), calcinations variables (calcination
temperature and calcination soaking duration). Therefore, the objectives of this
1. To synthesize single-phase -TCP powders by a wet
precipitation method and a hydrothermal method.
2. To investigate the optimum reaction parameters (stirring speed,
stirring duration) and calcination condition (calcination
temperature, soaking time) to form a single phase -TCP.
3. To study the mechanism of phase transformation of the
synthesized powder upon calcination.
4. To characterize the physical properties of single phase -TCP
powder such as density and morphology.
1.4 Research scope
In general, the research is divided into two parts which will be described
in more detail in chapter 3. The first part is the synthesis of -TCP using a wet
precipitation method from Ca(OH)2 and H3PO4 starting materials with a Ca/P
ratio of 1.5 The effect of reaction parameters (stirring speed, stirring duration)
and calcination conditions (calcination temperature, soaking time) were studied.
The characterization of the product powders were carried out using XRD, FTIR,
SEM and the density of powders were observed.
The second part is the synthesis of -TCP using a hydrothermal method
from the same Ca(OH)2 and H3PO4 staring material with a Ca/P ratio of 1.5. In
this part, the effect of stirring speed and calcination condition were studied. The
results of first part and second part were compared to understand the effect of
each method. The full detail of each method will be described in chapter 3,
however the methodology adopted in this research work can be summarized in
the flow charts shown in Figure 1.1 and 1.2
Figure 1. 1: Flow chart of the wet precipitation method (the first part).
H3PO4 solution Ca(OH)2 solution
Filtering and washing
Figure 1. 2: Flow chart of the hydrothermal method (the second part).
H3PO4 solution Ca(OH)2 solution
Filtering and washing
***Table of content CHAPTER 1 ....................................................................................................... 1
1.1 Introduction ............................................................................................... 1 1.2 Problem statement ................................................................................... 2 1.3 Objectives of research .............................................................................. 4 1.4 Research scope ........................................................................................ 5
***Table of content ............................................................................................. 8
LIST OF TABLE Table 1. 1 Prediction of market share of orthopedic biomaterials over the
world in 5 years 2007-2011 (Driscoll, 2006). ............................................... 1 LIST OF FIGURE Figure 1. 1 Flow chart of the wet precipitation method (the first part). ............ 6 Figure 1. 2 Flow chart of the hydrothermal method (the second part). ........... 7
2.1 Biomaterials The term biomaterials can be interpreted in two ways; first, as biological
materials such as tissue and blood; and second, as implant materials that
replace the function of the biological material (Park and Lake, 1992). According
to its legal definition as frequently referenced in the literature, a biomaterial is a
nonviable material used in a medical device, intended to interact with a
biological system (Williams, 1988). Thus, a biomaterial must always be
considered in its final fabricated and sterilized form. It was Williams, in 1988,
who coined the words biomaterial and biocompatibility to indicate the
biological performance of these materials. Thus, materials that are
biocompatible can also be considered as biomaterials.
In 1982, the National Institute of Health Consensus Development
Conference organized in America defined a biomaterial as any substance
(other than drug) or combination of substances, synthetic or natural in origin,
which can be used for any period of time, as a whole or as a part of a system
which treats, augments, or replace any tissue, organ, or function of the body
(The National Institute of Health Consensus Development Program: Clinical
Applications of Biomaterials website, 1982).
Biomaterials can broadly be classified as biological biomaterials and
synthetic biomaterials. Biological materials can be further classified into soft and
hard tissue types whilst synthetic materials can be further grouped into metallic,
polymeric, ceramic and composite biomaterials. Table 2.1 shows the various
classifications and some examples of biomaterials.
Table 2. 1: Classification of biomaterials (Hin, 2004)
I. Biological materials II. Synthetic biomedical materials
1. Soft tissue:
Skin, tendon, pericardium,
Ultra High Molecular Weight
Silicone, Polyurethane (PU),
2. Hard Tissue:
Bone, dentine, cuticle, etc
Stainless steel, Cobalt-based alloy
(Co-Cr-Mo), Titanium alloy (Ti-Al-
V), Gold, Platinum
Alumina (Al2O3), Zirconia (ZrO2),
phosphate [Ca3(PO4)2], Bioglass
Carbon Fiber (CF) composite such
as: CF/PEEK, CF/UHMWPE,
Synthetic materials are currently being used for biomedical applications.
Since they have different structures, they have varying properties and uses in
the body. These types of synthetic biomaterials will be presented in the next
2.2 Types of Synthetic Biomaterials
2.2.1 Metallic biomaterials
Metals have been used almost exclusively for load-bearing implants,
such as hip and knee prostheses, fracture fixation wires, pins, screws, and
plates (Dee et al., 2002). Metals have also been used as parts of the artificial
heart valves, e.g. such as vascular stents and pacemaker leads. Although pure
metals are sometimes used, alloys (metal containing two or more elements)
frequently provide improvement in material properties, such as strength and
corrosion resistance. Three alloy systems dominate biomedical metals: 316L
stainless steel, cobalt-chromium-molybdenum alloy, and pure titanium and
titanium alloy. The main consideration in selecting metals and alloys for
biomedical application are biocompatibility, appropriate mechanical properties,
corrosion resistance and reasonable cost.
The mechanical properties of materials are of great importance when
designing load-bearing orthopedic and dental implants. The mechanical
properties of a biomaterial can best be described by its modulus of elasticity,
tensile strength, elongation to failure and fracture toughness. Some mechanical
properties of metallic biomaterials are listed in Table 2.2. With a few
exceptions, the high ultimate tensile and fatigue strength of metals, compared to
ceramic and polymers make them the materials of Choi and Kumtace for
implants that carry mechanical loads.
The elastic moduli of the metals listed in Table 2.2 are at least seven
times greater than that of natural bone. This mismatch of mechanical properties
can cause stress shielding, a condition characterized by bone resorption (loss
of bone) in the vicinity of implants. This clinical complication arises because the
preferential distribution of mechanical loading through the metallic prosthesis
Table 2. 2: Selected properties of metallic biomaterials (Dee et al., 2002)
Materials Youngs modulus, E
Yield strength, y [MPa]
Tensile strength, UTS [MPa]
Fatigue limit, end [MPa]
Stainless steel 190 221-1,213 586-1,351 241-820
Co-Cr alloys 210-253 448-1,606 655-1,896 207-950
Titanium 110 485 760 300
Ti-6Al-4V 116 896-1,034 965-1,103 620
Natural bone 15-30 30-70 70-150 -
2.2.2 Ceramic and glass biomaterials
Ceramics, in general, can be defined as the art and science of making
and using solid articles composed of inorganic and nonmetallic materials for
functional applications. Typically, ceramics are fabricated by synthesizing
powders, followed by shaping and consolidation processes, which enable the
fabrication of objects of different shapes and sizes. Ceramics are refractory,
inorganic compounds made of metals and nonmetals such as O, N, C, S.
Exceptions to this general category include diamond, graphite, carbon
nanotubes, and pyrolized carbons (Kingery et al., 1976).
In recent years, ceramics and composites can also be used to augment
or replace various parts of the body, particularly the bone. Ceramics that can
be used for the body are called bioceramics. Their relative inertness to body
fluids, high compressive strength, and pleasing aesthetic appearance have led
to the use of ceramics in dentistry as dental crown. Some carbons have been
used as implant for blood interfacing application such as heart valves. Due to
their high specific strength as fibers and owing to their biocompatibility,
ceramics are also used as reinforcing components of composite implant
materials and for tensile loading applications such as tendons and ligaments.
Unlike metals and polymers, ceramics do not shear plastically due to the
ionic nature of the bonding and a minimum number of slips systems. Thus
ceramics are non ductile and are responsible for almost zero creep at room
temperature. Ceramics are susceptible to notches and cracks (micro-cracks)
since they do not undergo plastic deformation. Ceramics fracture elastically on
initiation of cracks. At the crack tip, stress could be many times larger than the
stress in the material away from the tip, leading to stress concentration
weakening in the material (Billotte, 2000).
In general, ceramics are hard: diamond is the hardest, with a hardness
index of 10 on the Mohs scale followed by alumina (Al2O3, hardness 9) and
quartz (SiO2, hardness 8). Other characteristics are: high melting temperatures
and low conductivity of electricity and heat.
The desired properties of bioceramics are:
Biofunctional for its lifetime in the host
Ceramics used in fabricating implants can be classified as biodegradable
or resorbable (non-inert); bioactive or surface reactive (semi-inert) and
nondegradable (relatively inert). Al2O3, ZrO2, Si3N4 and carbons are inert
bioceramics. Certain glass-ceramics and dense hydroxyapatite (HA) are semi-
inert (bioreactive) and calcium phosphates are degradable ceramics. Some Ca-
phosphates also contain alumina (AlCaP) which can be biodegradable.
Ceramics and glasses are also used as components of hip implants,
dental implants, middle ear implants and heart valves. Overall, however, these
biomaterials have been used less extensively than either metals or polymers.
Some ceramics that have been used for biomedical application are listed in
Table 2. 3: Ceramics used in biomedical application (Dee et al., 2002).
Ceramics Chemical formula Remarks
Alumina Al2O3 Bio-inert
Zirconia ZrO2 Bio-inert
Pyrolytic carbon Bio-inert
Bioglass Na2O.CaO.P2O3-SiO2 Bioactive
Hydroxyapatite (sintered at high temperature)
(sintered at low temperature)
Tricalcium phosphate Ca3(PO4)2 Biodegradable
The fundamental principle in classifying ceramic biomaterials is based on
chemical reactivity with the physiological environment (Figure 2.1). Relative
inert bioceramic, such as structural Al2O3, tend to exhibit inherently low levels of
reactivity which peak on the order of 104 day (over 250 years). Bioactive
ceramic, such as bioglass have a substantially higher level of reactivity peaking
on the order of 100 days. Resorbable or degradable bioceramics, such as
tricalcium phosphate, have even higher levels of reactivity peaking on the order
of 10 days. This broad spectrum of chemical behavior has led to a
corresponding range of engineering design materials (Hench, 1991).
Figure 2.1: Bioactivity spectrum for various bioceramic implants. (Hench, 1991).
The major drawbacks to the use of ceramics and glasses as implants are
their brittleness and poor tensile strength properties (see Table 2.4). Although
they can have outstanding strength when loaded in compression, ceramics and
glasses fail at low stresses when loaded in tension or bending. Among
biomedical ceramics, alumina has the highest mechanical properties, but its
tensile properties are still below those of metallic biomaterials. Additional
advantageous properties of alumina are its low coefficient of friction and wear
rate. As a consequence of these properties, alumina has been used as a
bearing surface in joint replacements.
Table 2. 4: Mechanical properties of ceramic biomaterial (Dee et al., 2002).
Materials Youngs modulus , E
Compressive strength, UCS
Tensile strength, UTS
Alumina 380 4500 350
Bioglass-ceramic 22 500 56-83
40-117 510-896 69-193
Pyrolytic carbon 18-28 517 280-560
The mechanical properties of calcium phosphates and bioactive glasses
make them unsuitable as load-bearing implants. Clinically, hydroxyapatite has
been used as a filler for bone defects and as implant in load-free anatomic sites
(for example, nasal septal bone and middle ear). In addition, hydroxyapatite has
been used as a coating on metallic orthopedic and dental implants to promote
their fixation in bone. In these cases, the underlying metal carries the load,
whereas the surrounding bone strongly bonds to hydroxyapatite.
2.2.3 Polymeric biomaterials
Polymers are the most widely used materials in biomedical applications.
They are the materials of Choi and Kumtace for cardiovascular devices as well
as for replacement and augmentation of various soft tissues. Polymers are also
used in drug delivery system, in diagnostic aids, and as a scaffolding material
for tissue engineering applications. Example of current applications include
vascular graft, heart valves, artificial hearts, breast implants, contact lenses,
intraocular lenses, components of extracorporeal oxygenators, dialyzers and
plasmapheresis units, coating for pharmaceutical tablets and capsules, sutures,
adhesives and blood substitutes. Examples of polymers and their uses are
given in Table 2.5.
Table 2. 5: Examples of biomedical application of polymers (Dee et al., 2002).
Polyethylene; polyvinylchloride (PVC); polyester; silicone
rubber; polyethylene terephthalate;
Orthopedic implant Ultra high molecular weight polyethylene (UHMWPE);
polymethyl methacrylate (PMMA)
Drug release Polylactide-co-glycolide
Tissue engineering Polylactic acid; polyglycolic acid; poly lactide-co-glycolide
The mechanical properties of polymers depend on several factors,
including the composition and structure of the macromolecular chains and their
molecular weights. Table 2.6 lists some mechanical properties of selected
polymeric biomaterials. Compared with metals and ceramics, polymers have
much lower strengths and moduli but they can be deformed to a greater extent
before failure. Consequently, polymers are generally not used in biomedical
applications that bear loads (such as body weight). Ultra high molecular weight
polyethylene (UHMWPE) is an exception, as it is used as a bearing surface in
hip and knee replacements. The mechanical properties of polymers, however,
are sufficient for numerous biomedical application (some of which are listed in
Table 2. 6: Mechanical properties of biomedical polymers (Dee et al., 2002).
Polymer Tensile strength,
Youngs Modulus, E
Polymethyl methacrylate (PMMA) 30 2.2 1.4
Nylon 6/6 76 2.8 90
Polyethylene terephthalate 53 2.14 300
Polylactic acid 28-50 1.2-3 2-6
Polypropylene 28-36 1.1-1.55 400-900
Polytetrafluoroethylene 17-28 0.5 120-350
Silicone rubber 2.8 Up to 10 160
Ultra high molecular weight
polyethylene (UHMWPE) 35 4-12 300
2.3 Calcium phosphate ceramics (CPC)
2.3.1 General properties of calcium phosphate ceramics:
As mentioned in the section 2.2.2, -TCP can be classified to the calcium
phosphate group. Thus, calcium phosphate will be focused in this section.
There are several forms of calcium phosphate. They typically form a family of
compounds called apatites. The name apatite was derived from apataw,
the Greek word to deceive, since it was confused with several other similar
looking minerals until chemical analysis conducted proved that calcium
phosphate composition is similar to enamel, dentin and bone (see Table 2.7).
There are several types of calcium phosphate, such as tricalcium
phosphate (TCP), hydroxyapatite (HA), dicalciumphosphate dihydrate (DCPD or
brushite), dicalcium phosphate anhydrous (DCPA or monetite). They exist in
different forms and phases depending on temperature, partial pressure of
waters and the presence of impurities (Hench, 1998). Different phases are used
in different applications depending upon whether a degradable or a bioactive
material is desired (Billotte, 2000). Table 2.8 summarized various phases of
calcium phosphate currently used in the biomedical industry. Table 2.9 presents
solubility of different phases of calcium phosphate in aqueous solution.
Table 2. 7: Comparison between enamel, dentin, bone and synthetic apatite
Element % Enamel Dentine Bone Synthetic apatite
Ca/P atomic ratio 1.62 1.59 1.61 1.667
Crystallinity good poor poor good
The mechanical properties of synthetic calcium phosphates vary
considerably (Table 2.10). The wide range in the properties of polycrystalline
calcium phosphates are due to the variations in their structure and
manufacturing processes. Depending on the final firing condition, calcium
phosphate can be hydroxyapatite or -TCP. In many instances, both types of
structures exist in the final product (Park and Lakes, 1992).
Table 2. 8: Various phases of calcium phosphate ceramics (Guelcher and
Hollinger and Hollinger, 2006).
Phases Chemical formulae
Hydroxyapatite (HA) Ca10(PO4)6(OH)2 Apatite 1.67
-Tricalcium phosphate (-TCP) Ca3(PO4)2 Whitlockite 1.5
-Tricalcium phosphate (-TCP) Ca3(PO4)2 Whitlockite 1.5
Dicalcium phosphate dihydrate
(DCPD) CaHPO4.2H2O Brushite 1.0
Dicalcium phosphate anhydrous
(DCPA) CaHPO4 Monetite 1.0
Table 2. 9: Solubility of different calcium phosphates (Schdmidt, 1993).
In water [g/l] In 0.1 Ml HCl
HA Insoluble Soluble
-TCP 0.02 Soluble
Brushite 0.3 Soluble
Monetite 0.2 Soluble
Table 2. 10: Physical properties of calcium phosphates (Park and Lakes, 1992)
Elastic modulus (GPa)
Compressive strength (MPa)
Bending strength (MPa)
Density (theoretical, g/cm3)
In addition, calcium phosphates are widely used in food and
pharmaceutical products, for instance as a calcium source in mineral tablets,
baking powders, cheese and meat products or as abrasive agents in
toothpaste. They are also used as tablets fillers/binders because of their good
binding properties, excellent flowability, low costs, chemical purity and relatively
few incompatibilities with pharmaceutical drugs. Table 2.11 shows the
commercially available calcium suitable for direct tablet. All these substances
are also available as fine powders for wet granulation, and food industry.
Table 2. 11: Calcium phosphates used for direct tablet (Schmidt and Herzog
and Herzog, 1993)
Formula Trade names Manufacturer
BK Ladenburd, Ladenburg, FRG.
Chemische Fabrik Budenheim,
Rhone-Poulenc, New York, USA.
E. Mendell Co., New York, USA.
Chemische Fabrik Budenheim.
Chemische Fabrik Budenheim.
E. Mendell Co.
Ca10(PO4)6(OH)2 Tri-Cafos S.
Chemische Fabrik Budenheim.
Among these calcium phosphate ceramics, bioresorbable or
biodegradable ceramics are most interesting. The concept of degradable
ceramics as bone substitutes was introduced in 1969 by Hentrich. However,
long before this plaster of paris was already being used as a bone substitute.
(Peltier, 1957). Degradable ceramics, as the name implies, degrade upon
implantation in the host and are slowly replaced by advancing tissue (such as
bone) (Guelcher and Hollinger and Hollinger, 2006). The rate of degradation
varies from material to material. Most bioresorbable ceramics except for
biocoral and plaster of paris are essentially variations of calcium phosphate.
Example of biodegradable bioceramics include: aluminum calcium
phosphorus oxides (AlCaP) (Mattie and Bajpai, 1988), glass fiber and their
composites (Alexander et al., 1987), coral [(Guillemin et al., 1989) and (Khavari
and Bajpai, 1993)]. Typical uses of biodegradable ceramics are drug delivery
devices (Abrams and Bajpai, 1994) and for repair of damaged bone due to
disease or trauma (Scheidler and Bajpai, 1992). A drawback of calcium
phosphate ceramics is their complicated fabrication process and particularly
difficult shaping. Nevertheless, calcium phosphate ceramics have gained and
will keep a place in clinical practice, as an alternative for autologous bone
grafting and as base material for implantable teeth.
The ideal Ca/P ratio of hydroxyapatite is 1.67 and the calculated density
is 3.219g/cm3. Substitution of OH- ion with fluoride gives the apatite greater
chemical stability due to the closer coordination of fluoride (symmetric shape),
as compared to the hydroxyl (asymmetric, two atoms) by the nearest calcium.
This is why fluoridation of drinking water helps in resisting caries of the teeth.
(Park and Lakes, 1992).
Hard tissue such as bone, dentin, and dental enamel are natural
composites which contain hydroxyapatite (or a similar mineral), as well as
protein, other organic materials and water. Enamel is the stiffest hard tissue,
with an elastic modulus of 74 GPa, and containing the most mineral
hydroxyapatite. Dentin (E = 21 GPa) and compact bone (E = 12 to 18 GPa)
contain comparatively less mineral. The Poissons ratio for the mineral or
synthetic hydroxyapatite is about 0.27, which is close to that of bone (~ 0.3)
(Park and Lakes, 1992).
2.3.3 Tricalcium phosphate (TCP)
-TCP is the low-temperature phase in the CaO - P2O5 phase diagram.
-TCP transforms to -TCP at 1125oC and above this, up to 1430oC, -TCP is a
stable phase. Above 1430oC, the super -TCP form becomes stable until the
melting point of 1756oC The ideal Ca/P ratio of -TCP is 1.5 and the theoretical
density is 3.17 g/cm3 as reported by Guelcher and Hollinger and Hollinger
(2006). Research has shown that tricalcium phosphate degrades faster than
calcium phosphate, [Ca2P2O7], which also degrades faster than hydroxyapatite
According to Kalita et al., (2007) and Guelcher and Hollinger (2006), -
TCP does not form in aqueous system under normal laboratory conditions
except with the introduction of small amounts of Mg2+ ions. Kalita et al., (2007)
and Billotte (2003) also agree that crystallization of various salts of calcium
phosphate like hydroxyapatite and -TCP depends on Ca/P ratio, presence of
water, impurities and temperature. For instance, in a wet environment and at a
lower temperature (
substitutes in a granular form or a solid block. A multi-crystalline porous form of
-TCP has been used successfully to correct periodontal defects and augment
bone contours (Metsger et al., 1982). X-ray diffraction of -TCP powder shows
an average interconnected porosity of over 100m (Lemons and Niemann,
Since TCP is a degradable temporary bone space filler material, when
implanted, TCP will interact with body fluids to form hydroxyapatite as follow:
4Ca3(PO4)2 + 2H2O Ca10(PO4)6(OH)2 + 2Ca2+ + 2HPO42- (2.1)
This reaction will decrease the pH of the local solution and further
increase the solubility of TCP. Theoretically, degradable -TCP is an ideal
implant material. After implantation, TCP will degrade with time and be replaced
with natural tissues. It leads to the regeneration of tissue instead of their
replacement and thus solves the problem of interfacial stability. However, in
clinical applications, some limitations restrict the use of degradable TCP:
Firstly, the mechanical performance of an implant must match the repair
rate of body tissues. According to Legeros et al., (1995), Ducheyne et al.,
(1990), the order of relative solubility of -TCP, -TCP and HA had been
suggested as -TCP ~ -TCP and very much greater than HA. In order to use
for surgical implantation, the degradation rate of the implant must be controlled
very well. To solve this problem, a composite between bioactive (semi-solubility)
and bioresorbable (high solubility) was mixed together to control the
degradation rate, for instance the biphasic calcium phosphate (BCP) between
hydroxyapatite and -TCP.
Secondly, large quantities of the implant materials must be handled by
the body cells and as such the constituents of a degradable implant must be
metabolically acceptable. TCP implants dissolve by grain-boundary
degradation. The released grains may cause a potential metabolic problem
because of their size (Gross et al., 1988).
2.3.4 Trace element measurement of HA and -TCP for surgical implant
The concentration of trace elements in HA and -TCP shall be limited for
surgical implant purpose (see Table 2.12). In this research work, -TCP
powders synthesized satisfy the requirement of the ASTM F1088-04a standard.
The concentrations of trace elements in -TCP powders will be discussed in
Table 2. 12: Standard specification of HA and -TCP for surgical implant
Standard specification of HA and -TCP for surgical implant
Element Maximum concentration, [ppm] HA -TCP As 3 3 Cd 5 5 Hg 5 5 Pb 30 30
Standard ASTM F1185-03 ASTM F1088-04a
2.3.5 Thermal behaviour of calcium phosphate ceramic
Schmidt and Herzog (1993) studied the thermal behavior of calcium
phosphate. Four types of calcium phosphate were used for his study: (1)
(1)-Hardcover(2)-soft cover(3)-Table of content(4)-Chapter 1(5)-CHAPTER 2